Optimized ground states parameters for all the three osmium double perovskites.
In this chapter, Osmium-based double perovskites Ba2XOsO6(X = Mg, Zn, Cd) have been investigated for their magnetic structure, electronic, elastic, mechanical and thermodynamic belongings. These materials have been recently reported experimentally for their magnetic structure. Here, we report the first successful ab initio calculations on the physical properties of these materials. The structural optimization for these Ba2XOsO6(X = Mg, Zn, Cd) double perovskite compounds has been finalized within density functional theory via full potential linearized augmented plane wave (FP-LAPW) method. The structural investigation exposes the ferromagnetic phase stability of these compounds. The spin-polarized electronic and magnetic properties were calculated within generalized gradient approximation (GGA), Hubbard approximation (GGA+U) and modified Becke-Johnson approximation (mBJ). The electronic profile establishes the half-metallic nature for all the three compounds. The total spin magnetic moment was found to be an integer value of 2 μb. The elastic constants have been calculated and used to predict mechanical stuffs like Shear modulus (G), Poisson ratio (v) and anisotropic factor. The calculated B/G and Cauchy pressure (C12-C44) both characterize these materials as brittle. The thermodynamic parameters like heat capacity and Debye temperature have been predicted in the temperature range of 0–1000 K.
- Ba2XOsO6 (X = Mg
- mechanical behavior
The need of advanced materials with novel properties for industrial and technological use has strained the material community to have a deep and appropriate understanding of the periodic table elements, along with their combinations. Therefore, materials community consequently observes the vital changes in innovative designing of novel materials. A tremendous increase in simulation power, along with algorithmic improvements in quantum theory allows one to have well-organized and exact quantum mechanical calculations. This has hence stretched the computing power to such extent that those properties of materials which were once observed extremely difficult are now easily being calculated with a great precision [1, 2]. From last few years work on perovskites especially double perovskites has geared up due to their vast technological applications and displaying multifunctional properties. The general formula of perovskites is looked as ABO3, where “A” and “B” are cations and “O” is oxygen anion. The charge of “A” and “B” cations can vary in the original Perovskite. Double perovskites are potential members of this diverse perovskite family having different structures, composition and properties. The double perovskite compounds having a general formula A2BB′O6 have benefited the material community because of great technological applications including spintronic materials, multi-ferroic materials, half-metallic materials, ferromagnetic materials, magneto-dielectric materials, magneto-optic materials, insulating ferrimagnetism [3, 4, 5, 6, 7, 8]. The double perovskite family exhibits a wide range of magnetic behaviors, like actually simple antiferromagnets presented by (Ba2LiOsO6), ferromagnets (Ba2MgReO6 and Ba2NaOsO6), spin singlet ground states for (Ba2YMoO6), and spin glasses(Sr2CaReO6) [9, 10, 11, 12, 13]. Osmium based double perovskites especially Sr2FeOsO6, SrFeCaOsO6, Ca2FeOsO6 have been extensively investigated for puzzling magnetic behavior [14, 15, 16, 17, 18, 19]. Perovskites with ABO3 structure like BaPuO3, SrPuO3, BaAmO3, SrAmO3, EuGaO3, EuInO3 etc. have been reported for spintronic applications [20, 21, 22, 23, 24]. Further materials like BaMoO3, SrMoO3, XReO3 (X = Rb, Cs, Tl), SnTaO3, PbMoO3 [25, 26, 27, 28] have been recently reported for fuel cell applications. Numerous investigations have also been reported on halide perovskites for solar cell applications like MAPbBr3 and MAPbI3 [29, 30, 31, 32, 33, 34, 35, 36].
Ba2XOsO6(X = Mg, Zn, Cd) cubic double perovskites have been recently reported in space group Fm-3 m (225). The complete details of the respective experimental lattice parameters are given in Table 1. The Ba atoms are located at 8c (1/4, 1/4, 1/4) of the unit cell, X atoms are at position 4b (0.5, 0.5, 0.5), Os atoms are positioned at 41a (0, 0, 0) and O atoms at 24e (X, 0, 0) (X = 0.233, 0.238, 0.234) respectively for Mg, Zn, Cd . Further double perovskites of the variant A2BB′O6 like Ba2MgReO6, Sr2MnTaO6, Ba2InTaO6 and many more have also been reported for electronic, magnetic, mechanical, optical, thermoelectric and thermodynamic investigations [38, 39, 40, 41, 42, 43, 44, 45, 46, 47]. As far Ba2XOsO6(X = Mg, Zn, Cd) compounds are concerned which belongs to the same variant not much attention has been paid towards these perovskites so far, regarding the above mentioned characteristic properties. Hence, in the present work an attempt to predict the properties for these double perovskite has been made and to check out their potential applications. The most successful density functional theory (DFT) has been employed for the investigation of magnetic, electronic, elastic, mechanical and thermo-physical behavior. For the investigation of thermo-physical behavior quasi harmonic Debye model [48, 49] has been used for the prediction of important parameters like specific heat, thermal expansion, Debye temperature, Grüneisen parameter etc.
|Lattice Constant||8.1548||8.07 |
|Mg, Zn, Cd-O||2.11||2.15||2.18|
|Ba, Mg, Zn, Cd||3.53||3.55||3.62|
|Os-Mg, Zn, Cd||4.07||4.10||4.19|
2. Computational details
The computational technique used during the calculations process is based on full-potential linearized augmented plane wave (FP-LAPW)  method based upon density functional theory (DFT)  as employed in WIEN2K. For structural optimization generalized gradient approximation (GGA) scheme of Perdew, Burke and Ernzerhof (PBE)  has been used. For electronic and magnetic calculations in addition to (GGA), Hubbard approximation (GGA + U)  and modified Becke-Johnson (mBJ)  has been used. For GGA + U approach the incorporation U- term can be done by various methods [54, 55]. In the present work we have used self-interaction correction method (SIC)  as implemented in WIEN2K. The value of Ueff was varied from 1 to 5 eV and J was set to 0, so as to properly adjust the Os-d in density of states. The final U value used throughout the calculations was set to 2.00 eV . For precise energy convergence the value of RMTKmax was taken 7, where RMT is the small atomic radius in unit cell and Kmax denotes the size of the largest
where E(V), P(V), are the total energy per unit cell, the constant hydrostatic pressure and Debye temperature respectively and is the vibration term written as;
in equation represents the Debye integral, N is the number of atoms per formula unit, the Boltzmann’s constant. The Debye temperature is expressed as;
In the above equation represents the adiabatic bulk modulus, M is the molecular mass per unit cell, the bulk modulus is expressed by
The non-equilibrium Gibbs function G*(V, P, T) can be minimized with respect to volume V;
Solution of Eq. (5) gives a detailed information about the thermodynamic quantities like thermal expansion heat capacity at constant volume CV, heat capacity at constant pressure CP, given respectively by;
In Eq. (8) represents the Grüneisen parameter, which is approximated as
3. Results and discussion
3.1 Structural properties
The optimized volume for all the three compounds has been made by fitting the total energy as a function of its cell volume using Birch–Murnaghan’s equation of state . Marjerrison et al.  have recently reported all the three compounds in cubic B1-phase space group Fm-3 m (225). The Ba atoms are located at position 8c (0.25, 0.25, 0.25), Mg, Zn, Cd at 4b (0.5, 0.5, 0.5), Os at 4a (0, 0, 0) and O atoms are sited at24e (X, 0, 0) (X = 0.233, 0.238, 0.234) respectively for Mg, Zn, Cd. The geometry and structural optimization has been carried in Non-magnetic (NM), ferromagnetic (FM), and anti-ferromagnetic (AFM) phases. The ground state energy was found lowest for all the three compounds in the ferromagnetic phase as presented in Figure 1(a–c), and thus a stable configuration.
The optimized ground state lattice constants are close to available experimental and theoretical results. The ground state parameters like bulk modulus (B0), lattice constant () pressure derivatives of bulks modulus and energy are grouped in Table 1.
3.2 Elastic and mechanical properties
In the present work the Charpin method has been employed for the calculation of elastic constants Cij (C11, C12, C44) values as implemented in WIEN2K. The values of elastic constants were obtained by calculating the total energy as a function of volume-conserving strains. The value of the elastic constants and mechanical properties are summed up in Table 2. The calculated values of elastic constants properly satisfy the criteria for cubic elastic constants and ensures the stability C11–C12 > 0, C11 > 0, C44 > 0, (C11 + 2C12) > 0, C12 < B < C11 . The Poisson’s ratio (
|Tm||2105 ± 300||2100 ± 300||1925 ± 300|
Zener anisotropy factor ‘A’ is the property of a material to show altered characteristic in various direction of its structure. As per this a material is isotropic if and only if ‘A’ factor has unit value or otherwise anisotropic. The calculated value of ‘A’ for the compound was found to 0.975, 1.08, 0.83 which is less than unity for Ba2MgOsO6 and Ba2CdOsO6 and greater than unity for Ba2ZnOsO6, hence in all the three cases deviating from unity, thus the materials will present anisotropic nature. Poisson’s ratio (ν) describes the nature of bonding forces. The upper and lower limits of Poisson’s ratio are 0.25 and 0.50 [20, 21, 22, 23, 24]. The (ν) value varies from material to material. For covalent materials, (ν) has a typical value of 0.1, for ionic materials (ν) = 0.25 and for metallic materials the value (ν) =0.33. The value of Poisson’s ratio for Ba2XOsO6(X = Mg, Zn, Cd) was calculated to be 0.261, 0.281 and 0.287respectively, which lies close to 0.25 and hence suggest a higher ionic behavior as inter-atomic bonding for these compounds. The obtained values of elastic constants have also been used to predict, one important thermodynamic parameter known as melting temperature [26, 27, 28]. The calculated value of melting temperature was found 2100 ± 300, 2105 ± 300, 1925 ± 300 K respectively for Ba2XOsO6(X = Mg, Zn, Cd). The calculated values of elastic constants, mechanical properties including melting temperature are grouped in Table 2.
3.3 Electronic and magnetic properties
For electronic structure calculations spin resolved band structure and density of states have been plotted using different correlation potentials. GGA calculated lattice parameter has been used to plot band structure and density of states within GGA, GGA + U and mBJ. These band structures and density plots usually deliver a decent understanding of the electronic contour of a material. The combination of different methods for band structure and density of state plots has been done as to understand the variation of results within different correlations. Figures 2(a–c), 3(a–c) and 4(a–c) represent the spin included band structures within GGA, GGA + U and mBJ respectively for Ba2XOsO6(X = Mg, Zn, Cd).
It is clear from these figures that the band profile for all the three compounds at the Fermi level is almost similar for all the approximation, presenting 100% of spin polarization. The Fermi level is set at 0 eV, separating the valance band maximum (VBM) from the conduction band minimum (CBM) in all figures. For spin up states the Fermi level remains fully occupied presenting metallic nature for all the three compounds and for spin down states the Fermi level remains completely vacant falling in a gap and thus generating a gap between(VBM) and (CBM), presenting the semi-conducting nature for the compounds. In case of Ba2MgOsO6 within GGA, GGA + U and mBJ respectively, the (VBM) lies on symmetry points ‘Γ’ at −1.30 eV, −1.1 eV and −1.3 eV, and CBM lies on symmetry point ‘X’ at 0.001, 0.7 and 1.2 eV respectively within GGA, GGA + U and mBJ. Hence in all the three cases the (VBM) and (CBM) lie on ‘Γ’ and X point making the compound indirect band gap semi-conductor in spin down states. The band gap value changes as we apply U and mBJ, the value of band gap found in GGA, GGA + U and mBJ are 1.3, 1.8 and 2.5 eV respectively for Ba2MgOsO6. For Ba2ZnOsO6 the valance band maxima (VBM) lie on symmetry points ‘Γ’ at −1.40, −1.2, −1.4 eV respectively in GGA, GGA + U and mBJ, and the conduction band minimum (CBM) lies on symmetry point ‘X’ at 0.2, 0.7, and 1.0 eV respectively in GGA, GGA + U and mBJ, thus generating an indirect band gap of 1.6, 1.9 and 2.4 eV respectively for GGA, GGA + U and mBJ. Similarly for Ba2CdOsO6 the valance band maxima (VBM) lie on symmetry points ‘L’ at −1.00, −0.8, −0.9 eV respectively in GGA, GGA + U and mBJ, the conduction band minimum (CBM) lies on symmetry point ‘X’ at 0.5, 0.8, and 1.4 eV respectively in GGA, GGA + U and mBJ, thus generating an indirect band gap of 1.5, 1.6 and 2.3 eV respectively for GGA, GGA + U and mBJ. Thus from the band structure calculations 100% of spin polarization at Fermi level is observed. The compounds behave as metallic for spin up states and semi-conducting for spin down states. The overall band picture presents half-metallic nature for all the three compounds.
For the further explanation of the band picture, total density of states (TDOS) and partial density of states (PDOS) have been plotted. The spin included combined TDOS shown in Figure 5(a–c) disclose the same results as presented by band structure plots presenting metallic nature for spin up states and semi-conducting for spin down states for all the three approximations and hence overall half-metallic nature. The DOS peaks are found to increase in case of GGA + U and mBJ. The contribution to the TDOS picture has been represented by the partial contribution to the DOS diagram as depicted in Figure 6(a–c) for both spin up and down states within GGA + U. The (PDOS) has been plotted for (Ba-‘s’, ‘p’, ‘d’, ‘f’), (Mg- ‘s’, ‘p’, Zn-‘s’, ‘p’, ‘d’), (Cd-‘s’, ‘p’, ‘d’), (Os- ‘s’, ‘p’, ‘d’, ‘f’) and O-‘s’, ‘p’ states. From these figures. it is clear that the metallic nature in spin up states for the compound in all the approximations is due to the Os-‘d’ states which are present at Fermi level with a small contribution of O-‘p’ states hybridized with one another and in case of spin down these ‘d’- states of Os and ‘p’-states of O are pulled inside the conduction band, thereby generating a gap in spin down states. Thus the spin included band profile, TDOS and PDOS results display that Ba2XOsO6(X = Mg, Zn, Cd) all present half-metallic nature.
In order to check the magnetic nature of the compounds the total and partial magnetic moments have been calculated with GGA, GGA + U and mBJ. The total magnetic contribution is obtained as the summation of the partial moments of individual elements and the interstitial moments. The total magnetic moment obtained in all approximations is nearly same for all the compounds Ba2XOsO6(X = Mg, Zn, Cd) equal to an integer value 2 B shown in Table 3.The main contribution to the total magnetic moment is mostly found from Osmium atoms. The partial moment of Os element shows a great variation on the application of Hubbard U and mBJ potentials. Hence it is clear that the ferromagnetic nature and large value of total magnetic moment for Ba2XOsO6(X = Mg, Zn, Cd) is mainly due to Os atoms. The values of interstitial, partial and total magnetic moments are present in Table 3. Thus the large and integer value of magnetic moment of 2 B further verifies the half-metallic and ferromagnetic nature for Ba2MgOsO6. The integer value of magnetic moment is one of the criteria for the half-metallic nature of a compound [22, 23].
GGA + U
GGA + U
GGA + U
3.4 Thermodynamic properties
In order to check the thermodynamic behavior quasi-harmonic Debye approximation [26, 27, 28] has been employed to check the temperature and pressure variation of some noteworthy thermodynamic quantities like heat at constant volume (Cv), thermal expansion (α), Grüneisen parameter (γ), Debye temperature (θD) and also the bulk modulus variation for these double perovskites. The variation of these parameters has been investigated under pressure and temperature. The temperature has been varied from 0 to 1000 K and pressure ranges from 0 to 15 GPa, with the step size of 5 GPa pressure. In this range of temperature quasi harmonic Debye model remains unconditionally valid.
Figure 7(a–c) presents the variation of bulk modulus (B) with temperature at different pressure points respectively at 0, 5, 10, and 15 GPa. Our results present a clear decrease in bulk modulus with temperature and an increase is observed with pressure at different temperature values. The reason for this decrease of bulk modulus with temperature is that temperature reduces the hardness of a material, while pressure tends to increase the same.
Figure 8(a–c) depicts the variation of specific heat at constant volume (CV) with temperature and pressure. One can have a clear understanding from the Figure 8(a–c) that the escalation of CV is rapid under the lower temperature values of 0–300 K, but above 300 K a lethargic increase in CV can be seen, which further becomes constant at high temperature at about 800 K beyond which, it follows the famous Dulong-Petit limit . This variation of CV for solids is a common observation. The calculated value of CV at 300 K and 0 GPa of pressure for Ba2XOsO6(X = Mg, Zn, Cd) was found to be 223.89, 223.16, 225.04 J mol−1 K respectively.
Figure 9(a–c) shows the pressure and temperature dependence of thermal expansion coefficient, ‘α’ respectively for Ba2XOsO6(X = Mg, Zn, Cd). It is clear from the figure that the value of ‘α’ increase with increasing temperature, the increase in ‘α’ is found to be rapid under low temperatures values and under higher temperatures values a sluggish increase in ‘α’ is observed. The main reason for the sluggish increase of ‘α’ under high temperature values may be the saturation of ‘α’ beyond 300 K. Pressure has a reverse effect on ‘α’, increasing pressure decreases the ‘α’. Under high pressure values ‘α’ falls rapidly, same as the increase is observed under low temperatures.
Grüneisen parameter (γ) describes the variation in vibrational frequency of a lattice under the influence of temperature and pressure . Pressure and temperature variation of (γ) for Ba2XOsO6(X = Mg, Zn, Cd) is plotted in Figure 10(a–c). The value of (γ) increases with increasing temperature and under pressure a reverse is observed, pressure decreases the value of (γ) and has a lowest value at 15 GPa of pressure. The predicted value of (γ) at 300 K and 0 GPa of pressure is 2.088, 1.965, 2.099 respectively for Ba2XOsO6(X = Mg, Zn, Cd).
Debye temperature (
Ab initio calculations on electronic structure, magnetic, elastic, mechanical and thermodynamic properties of cubic double perovskite oxides Ba2XOsO6 (X = Mg, Zn, Cd) Ba2ZnOsO6 have been reported within density functional theory via full potential linearized augmented plane wave (FP-LAPW) method. The structural investigation reveals the ferromagnetic phase stability for these compounds. The spin polarized electronic and magnetic properties were calculated within generalized gradient approximation (GGA), Hubbard approximation (GGA + U) and mBJ (modified Becke-Johnson approximation). The electronic profile establishes half-metallic nature for these compounds and hence can strength the modern technological domain in terms of spintronic materials. The calculated total spin magnetic moment was found equal to 2 μB for all the three compounds. Thus these materials are also looked for magnetic materials. The elastic constants have been calculated and used to predict mechanical stuffs like Shear modulus (G) Poisson ratio (ν) and anisotropic factor (A). The calculated B/G and Cauchy pressure (C12–C44) both characterize the material as brittle. The thermodynamic parameters like heat capacity and Debye temperature have also been predicted in the temperature range of 0–1000 K.
Pilania G, Balachandran PV, Kim C, Lookman T. Finding new perovskite halides via machine learning. Frontiers in Materials. 2016; 3:13285
Moore EA. Computational modelling of inorganic solids. Annual Reports on the Progress of Chemistry, Section A: Inorganic Chemistry. 2008; 104:46
Kobayashi KI, Kimura T, Sawada H, Terakura K, Tokura Y. Room-temperature magnetoresistance in an oxide material with an ordered double-perovskite structure. Nature. 1998; 395:677
Iliev MN, Padhan P, Gupta A. Temperature-dependent Raman study of multiferroic Bi2NiMnO6 thin films. Physical Review B. 2008; 77:172303
Fiebig M, Lottermoser T, Frohlich D, Goltsev AV, Pisarev RV. Observation of coupled magnetic and electric domains. Nature. 2002; 419:818
Das H, De Raychaudhury M, Saha-Dasgupta T. Moderate to large magneto-optical signals in high Tc double perovskites. Applied Physics Letters. 2008; 92:201912
Krockenberger Y, Mogare K, Reehuis M, Tovar M, Jansen M, Vaitheeswaran G, et al. Sr2CrOsO6: End point of a spin-polarized metal-insulator transition by 5d band filling. Physical Review B. 2007; 75:020404
Feng HL, Arai M, Matsushita Y, Tsujimoto Y, Guo YF, Sathish CI, et al. High-temperature ferrimagnetism driven by lattice distortion in double perovskite Ca2FeOsO6. Journal of the American Chemical Society. 2014; 136:3235
Stitzer KE, Smith MD, Loye HCZ. Crystal growth of Ba2MOsO6 (M = Li, Na) from reactive hydroxide fluxes. Solid State Sciences. 2002; 4:311
Aharen T, Greedan JE, Bridges CA, Aczel AA, Rodriguez J, MacDougall G, et al. Magnetic properties of the geometrically frustrated S = 1/2 antiferromagnets, La2LiMoO6 and Ba2YMoO6, with the B-site ordered double perovskite structure. evidence for a collective spin singlet ground state. Physical Review B. 2010; 81:224409
de Vries MA, Mclaughlin AC, Bos J-WG. Valence bond glass on an fcc lattice in the double perovskite Ba2YMoO6. Physical Review Letters. 2010; 104:177202
Carlo JP, Clancy JP, Aharen T, Yamani Z, Ruff JPC, Wagman JJ, et al. Triplet and in-gap magnetic states in the ground state of the quantum frustrated fcc antiferromagnet Ba2YMoO6. Physical Review B. 2011; 84:100404
Wiebe CR, Greedan JE, Luke GM, Gardner JS. Spin-glass behavior in the S=1/2 fcc ordered perovskite Sr2CaReO6. Physical Review B. 2002; 65:144413
Morrow R, Freeland JW, Woodward PM. Probing the links between structure and magnetism in Sr(2-x)Ca(x)FeOsO6 double perovskites. Inorganic Chemistry. 2014; 53:7983
Paul AK, Reehuis M, Ksenofontov V, Yan B, Hoser A, Tobbens DM, et al. Lattice instability and competing spin structures in the double perovskite insulator Sr2FeOsO6. Physical Review Letters. 2013; 111:167205
Kanungo S, Yan B, Jansen M, Felser C. Ab-initio study of low-temperature magnetic properties of double perovskite Sr2FeOsO6. Physical Review B. 2014; 89:214414
Paul AK, Jansen M, Yan BH, Felser C, Reehuis M, Abdala PM. Synthesis, crystal structure, and physical properties of Sr2FeOsO6. Inorganic Chemistry. 2013; 52:6713
Ghimire MP, Hu X. Half metal transition driven by doping effects in osmium double perovskite. arXiv preprintarXiv. 2014; 1408:1771
Wang H, Zhu S, Ou X, Nu H. Ferrimagnetism in the double perovskite Ca2FeOsO6: A density functional study. Physical Review B. 2014; 90:054406
Dar SA, Srivastava V, Sakalle UK, Pagare G. Insight into structural, electronic, magnetic, mechanical, and thermodynamic properties of actinide perovskite BaPuO3. Journal of Superconductivity and Novel Magnetism. 2018; 31(10):3201
Dar SA, Srivastava V, Sakalle UK, Pagare G. First-principles investigation on electronic structure, magnetic,mechanical and thermodynamic properties of SrPuO3 perovskite oxide. Materials Research Express. 2018; 5:026106
Dar SA, Srivastava V, Sakalle UK, Khandy SA, Gupta DC. A DFT study on structural, electronic mechanical and thermodynamic properties of 5f-electron system BaAmO3. Journal of Superconductivity and Novel Magnetism. 2018; 31(01):141
Dar SA, Srivastava V, Sakalle UK. A First-principles calculation on structural, electronic, magnetic, mechanical, and thermodynamic properties of SrAmO3. Journal of Superconductivity and Novel Magnetism. 2017; 30(11):3055
Dar SA, Srivastava V, Sakalle UK, Parey V, Pagare G. DFT investigation on electronic, magnetic, mechanical and thermodynamic properties under pressure of some EuMO3 (M = Ga, In) perovskites. Materials Research Express. 2017; 4:106104
Dar SA, Srivastava V, Sakalle UK. A combined DFT and post-DFT investigation on cubic XMoO3 (X = Sr, Ba) perovskite oxides. Materials Research Express. 2017; 4:086304
Zhao S, Wei Z, Dar SA. Insight into the Structural, Electronic, Elastic, Mechanical, and Thermodynamic Properties of XReO3 (X = Rb, Cs, Tl) Perovskite Oxides: A DFT Study. Zeitschrift für Naturforschung A. 2019. DOI: 10.1515/zna-2019-0019
Dar SA, Srivastava V, Sakalle UK. High pressure and high temperature investigation of metallic perovskite SnTaO3. Journal of Molecular Modeling. 2018; 24:52
Dar SA, Srivastava V, Sakalle UK. Ab initio high pressure and temperature investigation on cubic PbMoO3 perovskite. Journal of Electronic Materials. 2017; 46(12):6870
Cao K, Li H, Liu S, Cui J, Shen Y, Wang M. MAPbI3-xBrx mixed halide perovskites for fully printable mesoscopic solar cells with enhanced efficiency and less hysteresis. Nanoscale. 2016; 8:8839-8846
Chen L-C, Weng C-Y. Optoelectronic Properties of MAPbI3 Perovskite/Titanium Dioxide Heterostructures on Porous Silicon Substrates for Cyan Sensor Applications. Nanoscale Research Letters. 2015; 10:404
Colella S, Mosconi E, Fedeli P, Listorti A, Gazza F, Orlandi F, et al. MAPbI3-xClx mixed halide perovskite for hybrid solar cells: The role of chloride as dopant on the transport and structural properties. Chemistry of Materials. 2013; 25:4613-4618
Ding J, Zhao Y, Du S, Sun Y, Cui H, Zhan X, et al. Polarization-dependent optoelectronic performances in hybrid halide perovskite MAPbX3 (X = Br, Cl) single-crystal photodetectors. Journal of Materials Science. 2017; 52:7907-7916
Najeeb MA, Ahmad Z, Shakoor RA, Alashraf A, Bhadra J, Thani NA, et al. Growth of MAPbBr3 perovskite crystals and its interfacial properties with Al and Ag contacts for perovskite solar cells. Optical Materials. 2017; 73:50
Lu H, Zhang H, Yuan S, Wang J, Zhan Y, Zheng L. An optical dynamic study of MAPbBr3 single crystals passivated with MAPbCl3/I3-MAPbBr3 heterojunctions. Physical Chemistry Chemical Physics. 2016:1-3
Chen L-C, Tseng Z-L, Huang J-K. A Study of inverted-type perovskite solar cells with various composition ratios of (FAPbI3)1-x(MAPbBr3)x. Nanomaterials. 2016; 6:183
Yuan S, Wang J, Yang K, Wang P, Zhang X, Zhan Y, et al. High efficiency MAPbI3-xClx perovskite solar cell via interfacial passivation. Nanoscale. 2018; 10:18909-18914
Marjerrison CA, Thompson CM, Sharma AZ, Hallas AM, Wilson MN, Munsie TJS, et al. Magnetic ground states in the three Os6+ (5d2) double perovskites Ba2MOsO6 (M=Mg, Zn, and Cd) from Néel order to its suppression. Physical Review B. 2016; 94:134429
Dar SA, Srivastava V, Sakalle UK, Pagare G. Insight into electronic structure, magnetic, mechanical and thermodynamic properties of double perovskite Ba2MgReO6: A first-principles investigation. Computational Condensed Matter. 2018; 14:137-143
Merabet B, Alamri H, Djermouni M, Zaoui A, Kacimi S, Boukortt A, et al. Optimal bandgap of double perovskite La-substituted Bi2FeCrO6 for Solar Cells: An ab initio GGA+U Study. Chinese Physics Letters. 2017; 34(1):016101
Dar SA, Srivastava V, Sakalle UK. Structural, elastic, mechanical, electronic, magnetic, thermoelectric and thermodynamic investigation of half metallic double perovskite oxide Sr2MnTaO6. Journal of Magnetism and Magnetic Materials. 2019; 484:298-306
Sahnoun O, Bouhani-Benziane H, Sahnoun M, Driz M. Magnetic and thermoelectric properties of ordered double perovskite Ba2FeMoO6. Journal of Alloys and Compounds. 2017; 714:704
Dar SA, Sharma R, Srivastava V, Sakalle UK. Investigation on the electronic structure, optical, elastic, mechanical, thermodynamic and thermoelectric properties of wide band gap semiconductor double perovskite Ba2InTaO6. RSC Advances. 2019; 9:9522
Dar SA, Srivastava V, Sakalle UK. Ab-initio DFT based investigation of double perovskite oxide Ba2CdOsO6 with cubic structure. Computational Condensed Matter. 2019; 18:e00351
Thompson CM, Marjerrison CA, Sharma AZ, Wiebe CR, Maharaj DD, Sala G, et al. Frustrated magnetism in the double perovskite La2LiOsO6: A comparison with La2LiRuO6. Physical Review B. 2016; 93:014431
Dar SA, Srivastava V, Sakalle UK, Parey V, Pagare G. A combined DFT, DFT+U and mBJ investigation on electronic structure, magnetic, mechanical and thermodynamics of double perovskite Ba2ZnOsO6. Materials Science and Engineering B. 2018; 236-237:217-224
Faizan M, Khan SH, Murtaza G, Khan A, Khenata R, Mahmood A, et al. Structural, elastic, electronic and magnetic properties of Ba2XOsO6 (X = Li, Na, Ca) double perovskites. Indian Journal of Physics. 2016; 90:1225
Dar SA, Srivastava V, Sakalle UK, Parey V. Electronic structure, magnetic, mechanical and thermo-physical behavior of double perovskite Ba2MgOsO6. European Physical Journal Plus. 2018; 133:64
Otero-de-la-Roza A, Abbasi-Perez D, Luaea V. Gibbs2: A new version of the quasiharmonic model code. II. Models for solid-state thermodynamics, features and implementation. Computer Physics Communications. 2011; 182:2232
Otero-de-la-Roza A, Luaea V. Equations of state and thermodynamics of solids using empirical corrections in the quasiharmonic approximation. Physical Review B. 2011; 84:184103
Wu Z, Cohen RE. More accurate generalized gradient approximation for solids. Physical Review B. 2006; 73:235116
Blaha P, Schwarz K, Madsen GKH, Kuasnicke D, Luitz J. Introduction to WIEN2K, an Augmented Plane Wane plus Local Orbitals Program for Calculating Crystal Properties. Vienna, Austria: Vienna University of Technology; 2001
Perdew JP, Burke K, Ernzerhof M. Generalized gradient approximation made simple. Physical Review Letters. 1996; 77:3865
Tran F, Blaha P. Accurate band gaps of semiconductors and insulators with a semilocal exchange-correlation potential. Physical Review Letters. 2009; 102:226401
Petukhov AG, Mazin II. Correlated metals and the LDA+U method. Physical Review B. 2003; 67:153106
Novak P, Kunes J, Chaput L, Pickett WE. Exact exchange for correlated electrons. Physica Status Solidi B: Basic Solid State Physics. 2006; 243:563
Aisimov VI, Solovye IV, Korotin MA, Czyzyk MT, Sawatzky GA. Density-functional theory and NiO photoemission spectra. Physical Review B. 1993; 48:16929
Hou YS, Xiang HJ, Gong XG. Lattice-distortion induced magnetic transition from low-temperature antiferromagnetism to high-temperature ferrimagnetism in double perovskites A2FeOsO6 (A = Ca, Sr). Scientific Reports. 2015; 5:13159
Monkhorst HJ, Pack JD. Special points for Brillouin-zone integrations. Physical Review B. 1976; 13:5188
Charpin T. A Package for Calculating Elastic Tensors of Cubic Phases Using WIEN. Paris, France: Laboratory of Geometrix F-75252; 2001
Birch F. The effect of pressure upon the elastic parameters of isotropic solids, according to Murnaghan’s theory of finite strain. Journal of Applied Physics. 1938; 9:279
Dimitrovska S, Aleksovska S, Kuzmanovski I. Prediction of the unit cell edge length of cubic A22+ BB’O6 perovskites by multiple linear regression and artificial neural networks. Central European Journal of Chemistry. 2005; 3(1):198
Mehl MJ, Klein BK, Papaconstantopoulos DA. (Intermetallic compounds); principle and practice. In: Westbrook JH, Fleischeir RL, editors. Principles. Vol. 1. John Wiley and Sons; 1995
Voigt W. Lehrbush der Kristallphysik. Leipzig: Taubner; 1928
Schreiber E, Anderson OL, Soga N. Elastic Constants and Measurements. New York: M.C Graw Hill; 1973
Hill R. The elastic behaviour of a crystalline aggregate. Proceedings of the Physical Society (London). 1952; 65:349
Pugh SF. Relations between the elastic moduli and the plastic properties of polycrystalline pure metals. Philosophical Magazine. 1954; 45:823
Petit AT, Dulong PL. Sur quelques points importants de la théorie de la chaleur. Annales de Chimie Physique. 1819; 10:395
Quiang L, Duo-Hui H, Qi-Long C, Fan-Hou W. Phase transition and thermodynamic properties of BiFeO3 from first-principles calculations. Chinese Physics B. 2013; 22:037101